 
data_2 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          
'B18 K10 O54 V12 (O H)6, 15(H2 O)' 
_chemical_formula_sum 
 'B18 H36 K10 O75 V12' 
_chemical_formula_weight          2433.10  
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'B'  'B'   0.0013   0.0007 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Orthorhombic 
_symmetry_space_group_name_H-M    Pbca 
_symmetry_space_group_name_Hall   '-P 2ac 2ab '
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x+1/2, -y, z+1/2' 
 '-x, y+1/2, -z+1/2' 
 'x+1/2, -y+1/2, -z' 
 '-x, -y, -z' 
 'x-1/2, y, -z-1/2' 
 'x, -y-1/2, z-1/2' 
 '-x-1/2, y-1/2, z' 
 
_cell_length_a                    18.212(2) 
_cell_length_b                    19.276(2) 
_cell_length_c                    19.306(2) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  90.00 
_cell_angle_gamma                 90.00 
_cell_volume                      6777.7(14) 
_cell_formula_units_Z             4 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        octahedron 
_exptl_crystal_colour             black 
_exptl_crystal_size_max           0.18 
_exptl_crystal_size_mid           0.16 
_exptl_crystal_size_min           0.13 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.349 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              4624 
_exptl_absorpt_coefficient_mu     2.329 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.6426 
_exptl_absorpt_correction_T_max   0.7208 
_exptl_absorpt_process_details     
 'Jacobson, R. (1998) Private communication'  
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Rigaku Mercury'
_diffrn_measurement_method        ω
_diffrn_detector_area_resol_mean  7.31  
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             41122 
_diffrn_reflns_av_R_equivalents   0.0248 
_diffrn_reflns_av_sigmaI/netI     0.0172 
_diffrn_reflns_limit_h_min        -22 
_diffrn_reflns_limit_h_max        22 
_diffrn_reflns_limit_k_min        -21 
_diffrn_reflns_limit_k_max        24 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        24 
_diffrn_reflns_theta_min          1.87 
_diffrn_reflns_theta_max          26.50 
_reflns_number_total              7024 
_reflns_number_gt                 6150 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1151P)²+34.4221P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.' 
_refine_ls_hydrogen_treatment     none
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7024 
_refine_ls_number_parameters      585 
_refine_ls_number_restraints      6 
_refine_ls_R_factor_all           0.0696 
_refine_ls_R_factor_gt            0.0621 
_refine_ls_wR_factor_ref          0.2029 
_refine_ls_wR_factor_gt           0.1940 
_refine_ls_goodness_of_fit_ref    1.197 
_refine_ls_restrained_S_all       1.197 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
V1 V 0.67377(5) 0.39566(4) 0.49826(5) 0.0158(2) Uani 1 1 d . . 1 
V2 V 0.57858(5) 0.38813(4) 0.62544(5) 0.0153(2) Uani 1 1 d . . 1 
V3 V 0.42786(5) 0.43424(4) 0.66719(4) 0.0151(2) Uani 1 1 d . . 1 
V4 V 0.51630(5) 0.56511(4) 0.67211(4) 0.0146(2) Uani 1 1 d . . 1 
V5 V 0.58083(5) 0.66489(4) 0.56928(5) 0.0148(2) Uani 1 1 d . . 1 
V6 V 0.67965(5) 0.54026(4) 0.56046(5) 0.0144(2) Uani 1 1 d . . 1 
O1 O 0.7570(2) 0.5628(2) 0.5956(2) 0.0289(9) Uani 1 1 d . . 1 
O2 O 0.6482(2) 0.62027(19) 0.50589(19) 0.0192(8) Uani 1 1 d . . 1 
O3 O 0.6152(3) 0.3458(2) 0.6894(2) 0.0314(10) Uani 1 1 d . . 1 
O4 O 0.6252(2) 0.7279(2) 0.6057(2) 0.0291(9) Uani 1 1 d . . 1 
O5 O 0.6965(2) 0.49093(19) 0.4729(2) 0.0205(8) Uani 1 1 d . . 1 
O6 O 0.5956(2) 0.3398(2) 0.5376(2) 0.0205(8) Uani 1 1 d . . 1 
O7 O 0.6543(2) 0.44509(19) 0.5842(2) 0.0194(8) Uani 1 1 d . . 1 
O8 O 0.4894(2) 0.64753(19) 0.6192(2) 0.0187(8) Uani 1 1 d . A 1 
O9 O 0.5287(2) 0.46619(19) 0.6664(2) 0.0199(8) Uani 1 1 d . . 1 
O10 O 0.52575(19) 0.70590(18) 0.48967(19) 0.0160(7) Uani 1 1 d . . 1 
O11 O 0.6043(2) 0.58050(19) 0.61936(19) 0.0187(8) Uani 1 1 d . . 1 
O12 O 0.64014(19) 0.37382(18) 0.40144(19) 0.0163(7) Uani 1 1 d . . 1 
O13 O 0.4762(2) 0.36021(19) 0.6175(2) 0.0194(8) Uani 1 1 d . . 1 
O14 O 0.3363(2) 0.42087(18) 0.61142(19) 0.0165(7) Uani 1 1 d . . 1 
O15 O 0.4140(2) 0.53428(19) 0.6668(2) 0.0185(8) Uani 1 1 d . . 1 
O16 O 0.5432(3) 0.1348(3) 0.6347(3) 0.0417(12) Uani 1 1 d . . 1 
O17 O 0.6721(3) 0.2800(2) 0.2151(2) 0.0396(12) Uani 1 1 d . . 1 
O18 O 0.5344(2) 0.5886(2) 0.7517(2) 0.0290(9) Uani 1 1 d . . 1 
O19 O 0.7489(2) 0.3515(2) 0.5077(2) 0.0289(9) Uani 1 1 d . . 1 
O20 O 0.4092(2) 0.4070(2) 0.7445(2) 0.0257(9) Uani 1 1 d . . 1 
O21 O 0.7920(2) 0.5478(2) 0.4066(2) 0.0257(9) Uani 1 1 d . . 1 
O22 O 0.1219(2) 0.3636(2) 0.5822(3) 0.0354(11) Uani 1 1 d . . 1 
O23 O 0.3665(2) 0.29937(19) 0.5870(2) 0.0186(8) Uani 1 1 d . . 1 
O24 O 0.6674(2) 0.3836(2) 0.2778(2) 0.0204(8) Uani 1 1 d . . 1 
O25 O 0.4691(2) 0.2348(2) 0.6224(2) 0.0252(9) Uani 1 1 d . B 1 
O26 O 0.2478(2) 0.3391(2) 0.5620(2) 0.0255(9) Uani 1 1 d . . 1 
O27 O 0.5721(2) 0.2165(2) 0.5488(2) 0.0230(8) Uani 1 1 d . B 1 
O28 O 0.3977(2) 0.71532(19) 0.6807(2) 0.0212(8) Uani 1 1 d . . 1 
O29 O 0.7157(2) 0.46723(18) 0.35252(19) 0.0174(7) Uani 1 1 d . C 1 
O30 O 0.58173(19) 0.26588(18) 0.43870(19) 0.0156(7) Uani 1 1 d . . 1 
B1 B 0.3272(3) 0.3588(3) 0.5635(3) 0.0176(11) Uani 1 1 d . . 1 
B2 B 0.5563(3) 0.2798(3) 0.5076(3) 0.0155(11) Uani 1 1 d . . 1 
B3 B 0.5281(4) 0.1973(3) 0.6024(3) 0.0223(12) Uani 1 1 d . B 1 
B4 B 0.6531(3) 0.4236(3) 0.3419(3) 0.0163(11) Uani 1 1 d . . 1 
B5 B 0.4451(3) 0.2979(3) 0.5842(3) 0.0169(11) Uani 1 1 d . . 1 
B6 B 0.7160(3) 0.5196(3) 0.4047(3) 0.0176(11) Uani 1 1 d . . 1 
B7 B 0.4166(3) 0.6809(3) 0.6138(3) 0.0157(11) Uani 1 1 d . . 1 
B8 B 0.6452(3) 0.3168(3) 0.2713(3) 0.0207(12) Uani 1 1 d . . 1 
B9 B 0.1940(4) 0.3842(3) 0.5786(4) 0.0241(13) Uani 1 1 d . . 1 
K1 K 0.72061(8) 0.21618(9) 0.56957(9) 0.0407(4) Uani 1 1 d . . 1 
K2 K 0.87155(12) 0.51869(10) 0.67332(10) 0.0548(5) Uani 1 1 d . . 1 
K3 K 0.80983(11) 0.37690(15) 0.23263(14) 0.0746(8) Uani 1 1 d . . 1 
K4 K 0.5174(2) 0.33520(18) 0.81294(18) 0.0719(10) Uani 0.70 1 d P . 1 
K5 K 0.2908(2) 0.31852(19) 0.72678(17) 0.1048(11) Uani 1 1 d . . 1 
O3W O 0.4160(5) 0.2423(5) 0.7522(4) 0.0290(19) Uani 0.50 1 d P . 1 
O2W O 0.5807(5) 0.4473(5) 0.8038(4) 0.032(2) Uani 0.50 1 d P D 1 
O4W O 0.2932(5) 0.1919(5) 0.6398(5) 0.0310(19) Uiso 0.50 1 d P . 1 
O6W O 0.7828(14) 0.5207(17) 0.2382(11) 0.077(5) Uani 0.60 1 d PU . 1 
O5W O 0.2943(6) 0.3842(7) 0.8535(5) 0.052(3) Uani 0.50 1 d P . 1 
O9W O 0.9826(5) 0.5673(5) 0.4993(5) 0.032(2) Uani 0.50 1 d P E 1 
O1W O 0.5000 0.5000 0.5000 0.158(8) Uani 1 2 d S F 1 
O12W O 0.8975(8) 0.3475(8) 0.5190(13) 0.106(8) Uani 0.50 1 d P . 1 
O11W O 1.0537(10) 0.6462(7) 0.4484(12) 0.098(7) Uani 0.50 1 d P . 1 
O8A O 0.8438(17) 0.3817(16) 0.3748(16) 0.071(8) Uiso 0.25 1 d P . 1 
O7W O 0.8783(15) 0.4805(17) 0.5215(16) 0.074(10) Uani 0.25 1 d P G 1 
O2W' O 0.5446(9) 0.4759(7) 0.8480(8) 0.079(5) Uani 0.50 1 d P H 2 
O4W' O 0.2557(6) 0.2183(5) 0.6168(5) 0.036(2) Uiso 0.50 1 d P I 2 
O8C O 0.8646(6) 0.4229(5) 0.4376(6) 0.038(2) Uiso 0.50 1 d P J 2 
O7W' O 0.9253(17) 0.5308(15) 0.5260(11) 0.058(7) Uani 0.25 1 d P K 2 
O8B O 0.8730(12) 0.4226(11) 0.3978(13) 0.042(5) Uiso 0.25 1 d P J 2 
O6W' O 0.807(3) 0.529(3) 0.253(2) 0.121(14) Uani 0.40 1 d PU L 2 
K4' K 0.4693(4) 0.2674(4) 0.7673(4) 0.0612(19) Uani 0.30 1 d P M 2 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
V1 O19 1.623(4) . ? 
V1 O6 1.940(4) . ? 
V1 O5 1.945(4) . ? 
V1 O7 1.946(4) . ? 
V1 O12 2.012(4) . ? 
V1 V2 3.0091(13) . ? 
V1 V6 3.0370(12) . ? 
V1 K1 3.820(2) . ? 
V2 O3 1.624(4) . ? 
V2 O9 1.928(4) . ? 
V2 O7 1.934(4) . ? 
V2 O13 1.947(4) . ? 
V2 O6 1.959(4) . ? 
V2 V3 2.9958(13) . ? 
V2 K4 3.923(4) . ? 
V3 O20 1.618(4) . ? 
V3 O13 1.931(4) . ? 
V3 O9 1.936(4) . ? 
V3 O15 1.945(4) . ? 
V3 O14 2.002(4) . ? 
V3 V4 2.9946(13) . ? 
V3 K5 3.539(3) . ? 
V3 K2 3.631(2) 6_557 ? 
V3 K4 3.771(3) . ? 
V4 O18 1.636(4) . ? 
V4 O11 1.922(4) . ? 
V4 O9 1.923(4) . ? 
V4 O8 1.951(4) . ? 
V4 O15 1.958(4) . ? 
V4 V5 3.0035(12) . ? 
V4 K3 3.556(2) 2_665 ? 
V5 O4 1.620(4) . ? 
V5 O2 1.935(4) . ? 
V5 O11 1.940(4) . ? 
V5 O8 1.953(4) . ? 
V5 O10 1.998(4) . ? 
V5 V6 3.0065(12) . ? 
V5 K1 3.7490(18) 8_765 ? 
V5 K3 3.816(3) 2_665 ? 
V6 O1 1.623(4) . ? 
V6 O11 1.943(4) . ? 
V6 O7 1.947(4) . ? 
V6 O2 1.953(4) . ? 
V6 O5 1.964(4) . ? 
V6 K3 3.693(2) 2_665 ? 
V6 K1 3.8510(19) 8_765 ? 
O1 K2 2.706(5) . ? 
O1 K1 3.027(5) 8_765 ? 
O1 K3 3.135(5) 2_665 ? 
O2 B1 1.468(7) 5_666 ? 
O2 K1 3.261(4) 8_765 ? 
O3 K4 2.984(6) . ? 
O4 K1 2.903(5) 8_765 ? 
O4 K3 3.389(6) 2_665 ? 
O5 B6 1.471(7) . ? 
O6 B2 1.478(7) . ? 
O6 K1 3.353(4) . ? 
O8 B7 1.477(7) . ? 
O10 B2 1.521(7) 5_666 ? 
O10 B5 1.524(7) 5_666 ? 
O11 K3 2.811(4) 2_665 ? 
O12 B7 1.506(7) 5_666 ? 
O12 B4 1.517(7) . ? 
O13 B5 1.475(7) . ? 
O14 B1 1.521(7) . ? 
O14 B6 1.523(7) 5_666 ? 
O14 K5 3.088(5) . ? 
O15 B4 1.476(7) 5_666 ? 
O15 K2 3.196(4) 6_557 ? 
O16 B3 1.385(8) . ? 
O16 K2 2.824(5) 8_755 ? 
O17 B8 1.385(7) . ? 
O17 K1 2.946(5) 7_565 ? 
O17 K5 3.089(7) 4_556 ? 
O17 K3 3.145(5) . ? 
O18 K3 2.936(5) 2_665 ? 
O19 K1 2.914(5) . ? 
O20 K4 2.748(5) . ? 
O20 K2 2.761(4) 6_557 ? 
O20 K5 2.770(5) . ? 
O21 B9 1.366(8) 5_666 ? 
O21 B6 1.487(7) . ? 
O22 B9 1.375(8) . ? 
O22 K4 2.831(6) 6_557 ? 
O23 B1 1.426(7) . ? 
O23 B5 1.433(7) . ? 
O23 K5 3.052(5) . ? 
O24 B8 1.356(7) . ? 
O24 B4 1.482(7) . ? 
O24 K3 2.739(4) . ? 
O24 K2 2.850(4) 2_664 ? 
O25 B3 1.350(8) . ? 
O25 B5 1.488(7) . ? 
O26 B9 1.348(8) . ? 
O26 B1 1.496(7) . ? 
O26 K1 2.799(5) 4_456 ? 
O26 K5 3.300(6) . ? 
O27 B3 1.360(8) . ? 
O27 B2 1.485(7) . ? 
O27 K1 2.733(4) . ? 
O28 B8 1.362(8) 5_666 ? 
O28 B7 1.491(6) . ? 
O28 K4 2.783(5) 3_656 ? 
O29 B6 1.427(7) . ? 
O29 B4 1.431(7) . ? 
O29 K3 3.366(5) . ? 
O30 B2 1.434(7) . ? 
O30 B7 1.443(7) 5_666 ? 
O30 K4 3.326(5) 7_565 ? 
B1 O2 1.468(7) 5_666 ? 
B1 K5 3.314(7) . ? 
B1 K1 3.530(6) 4_456 ? 
B2 O10 1.521(7) 5_666 ? 
B2 K1 3.448(6) . ? 
B3 K1 3.581(7) . ? 
B4 O15 1.476(7) 5_666 ? 
B4 K2 3.468(6) 2_664 ? 
B5 O10 1.524(7) 5_666 ? 
B6 O14 1.523(7) 5_666 ? 
B7 O30 1.443(7) 5_666 ? 
B7 O12 1.506(7) 5_666 ? 
B7 K4 3.506(7) 3_656 ? 
B8 O28 1.362(8) 5_666 ? 
B8 K3 3.300(7) . ? 
B9 O21 1.366(8) 5_666 ? 
B9 K1 3.487(7) 4_456 ? 
K1 O26 2.799(5) 4_556 ? 
K1 O4 2.903(5) 8_755 ? 
K1 O17 2.946(5) 7_566 ? 
K1 O1 3.027(5) 8_755 ? 
K1 O2 3.261(4) 8_755 ? 
K1 B9 3.487(7) 4_556 ? 
K1 B1 3.530(6) 4_556 ? 
K2 O20 2.761(4) 6_657 ? 
K2 O16 2.824(5) 8_765 ? 
K2 O24 2.850(4) 2_665 ? 
K2 O5W 2.995(12) 6_657 ? 
K2 O7W 3.02(3) . ? 
K2 O6W 3.17(2) 2_665 ? 
K2 O15 3.196(4) 6_657 ? 
K2 B4 3.468(6) 2_665 ? 
K2 V3 3.631(2) 6_657 ? 
K2 K3 4.034(3) 2_665 ? 
K2 K4 4.432(4) 6_657 ? 
K3 O8A 2.82(3) . ? 
K3 O11 2.811(4) 2_664 ? 
K3 O6W 2.82(3) . ? 
K3 O4W 2.813(9) 4_556 ? 
K3 O18 2.936(5) 2_664 ? 
K3 O3W 3.017(9) 4_556 ? 
K3 O1 3.135(5) 2_664 ? 
K3 O4 3.389(6) 2_664 ? 
K4 O2W 2.456(11) . ? 
K4 O28 2.783(5) 3_646 ? 
K4 O3W 2.827(10) . ? 
K4 O22 2.831(6) 6_657 ? 
K4 O11W 2.94(3) 2_665 ? 
K4 O30 3.326(5) 7_566 ? 
K4 B7 3.506(7) 3_646 ? 
K4 K2 4.431(4) 6_557 ? 
K5 O5W 2.755(12) . ? 
K5 O3W 2.755(11) . ? 
K5 O4W 2.963(10) . ? 
K5 O17 3.089(7) 4_456 ? 
K5 K3 3.863(5) 4_456 ? 
O3W K3 3.017(9) 4_456 ? 
O4W O8A 1.72(3) 4_456 ? 
O4W K3 2.813(9) 4_456 ? 
O6W K2 3.17(2) 2_664 ? 
O5W K2 2.995(12) 6_557 ? 
O12W O11W 1.10(3) 5_766 ? 
O11W O12W 1.10(3) 5_766 ? 
O11W K4 2.94(3) 2_664 ? 
O8A O4W 1.72(3) 4_556 ? 
O8C O8B 0.78(2) . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O19 V1 O6 106.5(2) . . ? 
O19 V1 O5 110.1(2) . . ? 
O6 V1 O5 141.14(17) . . ? 
O19 V1 O7 108.4(2) . . ? 
O6 V1 O7 78.69(16) . . ? 
O5 V1 O7 77.95(16) . . ? 
O19 V1 O12 104.57(19) . . ? 
O6 V1 O12 91.39(16) . . ? 
O5 V1 O12 91.62(16) . . ? 
O7 V1 O12 147.07(16) . . ? 
O19 V1 V2 111.65(17) . . ? 
O6 V1 V2 39.72(11) . . ? 
O5 V1 V2 111.94(12) . . ? 
O7 V1 V2 39.00(11) . . ? 
O12 V1 V2 124.94(11) . . ? 
O19 V1 V6 114.05(16) . . ? 
O6 V1 V6 112.36(12) . . ? 
O5 V1 V6 39.25(11) . . ? 
O7 V1 V6 38.73(11) . . ? 
O12 V1 V6 124.77(11) . . ? 
V2 V1 V6 75.05(3) . . ? 
O19 V1 K1 45.22(16) . . ? 
O6 V1 K1 61.33(12) . . ? 
O5 V1 K1 153.94(13) . . ? 
O7 V1 K1 100.19(12) . . ? 
O12 V1 K1 102.32(11) . . ? 
V2 V1 K1 77.93(4) . . ? 
V6 V1 K1 132.91(4) . . ? 
O3 V2 O9 105.9(2) . . ? 
O3 V2 O7 107.8(2) . . ? 
O9 V2 O7 93.56(16) . . ? 
O3 V2 O13 108.3(2) . . ? 
O9 V2 O13 78.24(16) . . ? 
O7 V2 O13 143.85(17) . . ? 
O3 V2 O6 110.8(2) . . ? 
O9 V2 O6 143.22(17) . . ? 
O7 V2 O6 78.52(16) . . ? 
O13 V2 O6 87.26(16) . . ? 
O3 V2 V3 108.72(17) . . ? 
O9 V2 V3 39.28(12) . . ? 
O7 V2 V3 126.55(12) . . ? 
O13 V2 V3 39.24(11) . . ? 
O6 V2 V3 121.26(12) . . ? 
O3 V2 V1 114.09(17) . . ? 
O9 V2 V1 124.68(12) . . ? 
O7 V2 V1 39.29(11) . . ? 
O13 V2 V1 120.08(12) . . ? 
O6 V2 V1 39.25(11) . . ? 
V3 V2 V1 137.15(4) . . ? 
O3 V2 K4 44.27(17) . . ? 
O9 V2 K4 71.95(12) . . ? 
O7 V2 K4 136.88(13) . . ? 
O13 V2 K4 74.24(13) . . ? 
O6 V2 K4 136.05(13) . . ? 
V3 V2 K4 64.45(5) . . ? 
V1 V2 K4 158.31(6) . . ? 
O20 V3 O13 108.29(19) . . ? 
O20 V3 O9 108.0(2) . . ? 
O13 V3 O9 78.43(16) . . ? 
O20 V3 O15 107.33(19) . . ? 
O13 V3 O15 142.18(16) . . ? 
O9 V3 O15 78.89(16) . . ? 
O20 V3 O14 106.19(19) . . ? 
O13 V3 O14 90.99(16) . . ? 
O9 V3 O14 145.77(16) . . ? 
O15 V3 O14 91.03(16) . . ? 
O20 V3 V4 110.94(16) . . ? 
O13 V3 V4 113.15(12) . . ? 
O9 V3 V4 38.95(11) . . ? 
O15 V3 V4 40.04(11) . . ? 
O14 V3 V4 125.01(11) . . ? 
O20 V3 V2 110.16(16) . . ? 
O13 V3 V2 39.62(11) . . ? 
O9 V3 V2 39.08(11) . . ? 
O15 V3 V2 114.32(11) . . ? 
O14 V3 V2 125.48(11) . . ? 
V4 V3 V2 76.45(3) . . ? 
O20 V3 K5 49.26(17) . . ? 
O13 V3 K5 90.96(13) . . ? 
O9 V3 K5 150.61(14) . . ? 
O15 V3 K5 122.34(13) . . ? 
O14 V3 K5 60.41(12) . . ? 
V4 V3 K5 154.15(6) . . ? 
V2 V3 K5 123.13(8) . . ? 
O20 V3 K2 45.90(15) . 6_557 ? 
O13 V3 K2 151.76(13) . 6_557 ? 
O9 V3 K2 97.55(12) . 6_557 ? 
O15 V3 K2 61.44(12) . 6_557 ? 
O14 V3 K2 106.18(11) . 6_557 ? 
V4 V3 K2 75.37(4) . 6_557 ? 
V2 V3 K2 128.32(5) . 6_557 ? 
K5 V3 K2 78.92(7) . 6_557 ? 
O20 V3 K4 40.42(17) . . ? 
O13 V3 K4 78.42(13) . . ? 
O9 V3 K4 75.91(13) . . ? 
O15 V3 K4 124.09(13) . . ? 
O14 V3 K4 134.14(13) . . ? 
V4 V3 K4 99.80(7) . . ? 
V2 V3 K4 69.78(7) . . ? 
K5 V3 K4 75.13(10) . . ? 
K2 V3 K4 73.52(6) 6_557 . ? 
O18 V4 O11 106.7(2) . . ? 
O18 V4 O9 107.7(2) . . ? 
O11 V4 O9 91.45(16) . . ? 
O18 V4 O8 108.5(2) . . ? 
O11 V4 O8 78.84(16) . . ? 
O9 V4 O8 143.79(17) . . ? 
O18 V4 O15 109.0(2) . . ? 
O11 V4 O15 144.37(17) . . ? 
O9 V4 O15 78.89(16) . . ? 
O8 V4 O15 88.91(16) . . ? 
O18 V4 V3 111.82(16) . . ? 
O11 V4 V3 124.18(12) . . ? 
O9 V4 V3 39.27(12) . . ? 
O8 V4 V3 122.29(12) . . ? 
O15 V4 V3 39.72(11) . . ? 
O18 V4 V5 111.38(16) . . ? 
O11 V4 V5 39.17(11) . . ? 
O9 V4 V5 123.48(12) . . ? 
O8 V4 V5 39.73(11) . . ? 
O15 V4 V5 122.16(12) . . ? 
V3 V4 V5 136.80(4) . . ? 
O18 V4 K3 54.86(16) . 2_665 ? 
O11 V4 K3 51.89(12) . 2_665 ? 
O9 V4 K3 103.08(13) . 2_665 ? 
O8 V4 K3 98.03(13) . 2_665 ? 
O15 V4 K3 163.70(13) . 2_665 ? 
V3 V4 K3 138.97(6) . 2_665 ? 
V5 V4 K3 70.58(6) . 2_665 ? 
O4 V5 O2 107.0(2) . . ? 
O4 V5 O11 107.6(2) . . ? 
O2 V5 O11 78.62(16) . . ? 
O4 V5 O8 109.8(2) . . ? 
O2 V5 O8 140.97(17) . . ? 
O11 V5 O8 78.37(16) . . ? 
O4 V5 O10 106.7(2) . . ? 
O2 V5 O10 90.45(15) . . ? 
O11 V5 O10 145.66(16) . . ? 
O8 V5 O10 91.11(15) . . ? 
O4 V5 V4 112.85(17) . . ? 
O2 V5 V4 112.43(12) . . ? 
O11 V5 V4 38.74(11) . . ? 
O8 V5 V4 39.68(11) . . ? 
O10 V5 V4 124.42(11) . . ? 
O4 V5 V6 108.98(17) . . ? 
O2 V5 V6 39.58(11) . . ? 
O11 V5 V6 39.31(11) . . ? 
O8 V5 V6 113.67(12) . . ? 
O10 V5 V6 124.97(11) . . ? 
V4 V5 V6 76.11(3) . . ? 
O4 V5 K1 47.19(16) . 8_765 ? 
O2 V5 K1 60.42(12) . 8_765 ? 
O11 V5 K1 90.44(12) . 8_765 ? 
O8 V5 K1 150.10(12) . 8_765 ? 
O10 V5 K1 112.40(11) . 8_765 ? 
V4 V5 K1 123.04(4) . 8_765 ? 
V6 V5 K1 68.49(4) . 8_765 ? 
O4 V5 K3 62.55(17) . 2_665 ? 
O2 V5 K3 95.62(12) . 2_665 ? 
O11 V5 K3 45.25(12) . 2_665 ? 
O8 V5 K3 90.05(12) . 2_665 ? 
O10 V5 K3 168.85(11) . 2_665 ? 
V4 V5 K3 61.49(5) . 2_665 ? 
V6 V5 K3 64.26(4) . 2_665 ? 
K1 V5 K3 63.32(5) 8_765 2_665 ? 
O1 V6 O11 105.1(2) . . ? 
O1 V6 O7 111.1(2) . . ? 
O11 V6 O7 94.06(16) . . ? 
O1 V6 O2 105.6(2) . . ? 
O11 V6 O2 78.09(16) . . ? 
O7 V6 O2 143.27(17) . . ? 
O1 V6 O5 110.7(2) . . ? 
O11 V6 O5 143.82(17) . . ? 
O7 V6 O5 77.50(16) . . ? 
O2 V6 O5 87.92(16) . . ? 
O1 V6 V5 106.38(16) . . ? 
O11 V6 V5 39.23(11) . . ? 
O7 V6 V5 126.70(12) . . ? 
O2 V6 V5 39.13(11) . . ? 
O5 V6 V5 121.94(12) . . ? 
O1 V6 V1 116.21(16) . . ? 
O11 V6 V1 124.94(12) . . ? 
O7 V6 V1 38.72(12) . . ? 
O2 V6 V1 120.07(12) . . ? 
O5 V6 V1 38.80(11) . . ? 
V5 V6 V1 137.28(4) . . ? 
O1 V6 K3 57.50(17) . 2_665 ? 
O11 V6 K3 48.50(12) . 2_665 ? 
O7 V6 K3 102.00(13) . 2_665 ? 
O2 V6 K3 99.16(12) . 2_665 ? 
O5 V6 K3 167.49(13) . 2_665 ? 
V5 V6 K3 68.57(5) . 2_665 ? 
V1 V6 K3 139.00(6) . 2_665 ? 
O1 V6 K1 48.38(16) . 8_765 ? 
O11 V6 K1 87.41(12) . 8_765 ? 
O7 V6 K1 158.61(12) . 8_765 ? 
O2 V6 K1 57.84(12) . 8_765 ? 
O5 V6 K1 113.08(12) . 8_765 ? 
V5 V6 K1 64.92(3) . 8_765 ? 
V1 V6 K1 147.45(4) . 8_765 ? 
K3 V6 K1 63.49(6) 2_665 8_765 ? 
V6 O1 K2 144.8(2) . . ? 
V6 O1 K1 108.0(2) . 8_765 ? 
K2 O1 K1 107.17(14) . 8_765 ? 
V6 O1 K3 96.61(19) . 2_665 ? 
K2 O1 K3 87.03(14) . 2_665 ? 
K1 O1 K3 80.23(13) 8_765 2_665 ? 
B1 O2 V5 130.4(3) 5_666 . ? 
B1 O2 V6 128.3(3) 5_666 . ? 
V5 O2 V6 101.29(17) . . ? 
B1 O2 K1 88.0(3) 5_666 8_765 ? 
V5 O2 K1 88.52(14) . 8_765 ? 
V6 O2 K1 91.69(14) . 8_765 ? 
V2 O3 K4 113.4(2) . . ? 
V5 O4 K1 108.6(2) . 8_765 ? 
V5 O4 K3 92.35(18) . 2_665 ? 
K1 O4 K3 77.85(12) 8_765 2_665 ? 
B6 O5 V1 129.2(3) . . ? 
B6 O5 V6 128.7(3) . . ? 
V1 O5 V6 101.95(18) . . ? 
B2 O6 V1 129.5(3) . . ? 
B2 O6 V2 129.4(3) . . ? 
V1 O6 V2 101.02(17) . . ? 
B2 O6 K1 81.1(3) . . ? 
V1 O6 K1 88.17(14) . . ? 
V2 O6 K1 106.61(16) . . ? 
V2 O7 V1 101.71(17) . . ? 
V2 O7 V6 143.3(2) . . ? 
V1 O7 V6 102.55(18) . . ? 
B7 O8 V4 128.1(3) . . ? 
B7 O8 V5 131.0(3) . . ? 
V4 O8 V5 100.59(17) . . ? 
V4 O9 V2 148.5(2) . . ? 
V4 O9 V3 101.78(18) . . ? 
V2 O9 V3 101.64(18) . . ? 
B2 O10 B5 112.5(4) 5_666 5_666 ? 
B2 O10 V5 122.6(3) 5_666 . ? 
B5 O10 V5 121.8(3) 5_666 . ? 
V4 O11 V5 102.09(17) . . ? 
V4 O11 V6 146.8(2) . . ? 
V5 O11 V6 101.46(17) . . ? 
V4 O11 K3 95.56(15) . 2_665 ? 
V5 O11 K3 105.39(17) . 2_665 ? 
V6 O11 K3 100.32(15) . 2_665 ? 
B7 O12 B4 113.7(4) 5_666 . ? 
B7 O12 V1 122.5(3) 5_666 . ? 
B4 O12 V1 121.7(3) . . ? 
B5 O13 V3 130.1(3) . . ? 
B5 O13 V2 128.8(3) . . ? 
V3 O13 V2 101.14(17) . . ? 
B1 O14 B6 113.6(4) . 5_666 ? 
B1 O14 V3 121.2(3) . . ? 
B6 O14 V3 122.3(3) 5_666 . ? 
B1 O14 K5 84.7(3) . . ? 
B6 O14 K5 117.5(3) 5_666 . ? 
V3 O14 K5 85.28(14) . . ? 
B4 O15 V3 130.7(3) 5_666 . ? 
B4 O15 V4 128.8(3) 5_666 . ? 
V3 O15 V4 100.24(17) . . ? 
B4 O15 K2 87.8(3) 5_666 6_557 ? 
V3 O15 K2 86.25(13) . 6_557 ? 
V4 O15 K2 102.05(15) . 6_557 ? 
B3 O16 K2 156.6(4) . 8_755 ? 
B8 O17 K1 147.2(4) . 7_565 ? 
B8 O17 K5 106.1(4) . 4_556 ? 
K1 O17 K5 98.74(16) 7_565 4_556 ? 
B8 O17 K3 83.9(3) . . ? 
K1 O17 K3 81.31(13) 7_565 . ? 
K5 O17 K3 76.58(16) 4_556 . ? 
V4 O18 K3 98.03(19) . 2_665 ? 
V1 O19 K1 111.5(2) . . ? 
V3 O20 K4 117.1(2) . . ? 
V3 O20 K2 109.2(2) . 6_557 ? 
K4 O20 K2 107.10(17) . 6_557 ? 
V3 O20 K5 104.5(2) . . ? 
K4 O20 K5 107.90(19) . . ? 
K2 O20 K5 110.98(17) 6_557 . ? 
B9 O21 B6 121.9(5) 5_666 . ? 
B9 O22 K4 137.3(4) . 6_557 ? 
B1 O23 B5 120.3(4) . . ? 
B1 O23 K5 87.6(3) . . ? 
B5 O23 K5 119.2(3) . . ? 
B8 O24 B4 121.3(4) . . ? 
B8 O24 K3 102.0(3) . . ? 
B4 O24 K3 117.2(3) . . ? 
B8 O24 K2 119.2(4) . 2_664 ? 
B4 O24 K2 101.7(3) . 2_664 ? 
K3 O24 K2 92.38(13) . 2_664 ? 
B3 O25 B5 121.9(4) . . ? 
B9 O26 B1 122.3(5) . . ? 
B9 O26 K1 109.4(4) . 4_456 ? 
B1 O26 K1 106.5(3) . 4_456 ? 
B9 O26 K5 91.3(4) . . ? 
B1 O26 K5 77.5(3) . . ? 
K1 O26 K5 150.57(17) 4_456 . ? 
B3 O27 B2 121.1(4) . . ? 
B3 O27 K1 118.1(4) . . ? 
B2 O27 K1 105.8(3) . . ? 
B8 O28 B7 121.3(4) 5_666 . ? 
B8 O28 K4 131.7(3) 5_666 3_656 ? 
B7 O28 K4 106.2(3) . 3_656 ? 
B6 O29 B4 121.4(4) . . ? 
B6 O29 K3 148.2(3) . . ? 
B4 O29 K3 90.2(3) . . ? 
B2 O30 B7 121.7(4) . 5_666 ? 
B2 O30 K4 132.3(3) . 7_565 ? 
B7 O30 K4 84.9(3) 5_666 7_565 ? 
O23 B1 O2 111.1(4) . 5_666 ? 
O23 B1 O26 106.7(4) . . ? 
O2 B1 O26 110.3(5) 5_666 . ? 
O23 B1 O14 112.6(5) . . ? 
O2 B1 O14 107.8(4) 5_666 . ? 
O26 B1 O14 108.4(4) . . ? 
O23 B1 K5 66.9(3) . . ? 
O2 B1 K5 173.2(4) 5_666 . ? 
O26 B1 K5 76.4(3) . . ? 
O14 B1 K5 68.1(3) . . ? 
O23 B1 K1 100.3(3) . 4_456 ? 
O2 B1 K1 67.4(3) 5_666 4_456 ? 
O26 B1 K1 49.5(2) . 4_456 ? 
O14 B1 K1 145.5(3) . 4_456 ? 
K5 B1 K1 119.08(18) . 4_456 ? 
O30 B2 O6 110.7(4) . . ? 
O30 B2 O27 106.3(4) . . ? 
O6 B2 O27 109.8(4) . . ? 
O30 B2 O10 112.5(4) . 5_666 ? 
O6 B2 O10 108.7(4) . 5_666 ? 
O27 B2 O10 108.7(4) . 5_666 ? 
O30 B2 K1 88.6(3) . . ? 
O6 B2 K1 73.9(3) . . ? 
O27 B2 K1 49.7(2) . . ? 
O10 B2 K1 154.9(3) 5_666 . ? 
O25 B3 O27 122.8(5) . . ? 
O25 B3 O16 119.6(5) . . ? 
O27 B3 O16 117.5(5) . . ? 
O25 B3 K1 140.8(4) . . ? 
O27 B3 K1 42.3(3) . . ? 
O16 B3 K1 88.5(4) . . ? 
O29 B4 O15 110.7(4) . 5_666 ? 
O29 B4 O24 106.6(4) . . ? 
O15 B4 O24 109.7(4) 5_666 . ? 
O29 B4 O12 112.7(4) . . ? 
O15 B4 O12 107.8(4) 5_666 . ? 
O24 B4 O12 109.3(4) . . ? 
O29 B4 K2 92.8(3) . 2_664 ? 
O15 B4 K2 67.1(3) 5_666 2_664 ? 
O24 B4 K2 53.6(2) . 2_664 ? 
O12 B4 K2 153.5(3) . 2_664 ? 
O23 B5 O13 110.5(4) . . ? 
O23 B5 O25 106.9(4) . . ? 
O13 B5 O25 109.7(4) . . ? 
O23 B5 O10 112.6(4) . 5_666 ? 
O13 B5 O10 108.3(4) . 5_666 ? 
O25 B5 O10 108.8(4) . 5_666 ? 
O29 B6 O5 111.4(4) . . ? 
O29 B6 O21 106.2(4) . . ? 
O5 B6 O21 109.9(5) . . ? 
O29 B6 O14 112.7(5) . 5_666 ? 
O5 B6 O14 108.4(4) . 5_666 ? 
O21 B6 O14 108.2(4) . 5_666 ? 
O30 B7 O8 109.9(4) 5_666 . ? 
O30 B7 O28 107.2(4) 5_666 . ? 
O8 B7 O28 109.9(4) . . ? 
O30 B7 O12 112.0(4) 5_666 5_666 ? 
O8 B7 O12 109.0(4) . 5_666 ? 
O28 B7 O12 108.8(4) . 5_666 ? 
O30 B7 K4 70.9(3) 5_666 3_656 ? 
O8 B7 K4 91.9(3) . 3_656 ? 
O28 B7 K4 49.6(2) . 3_656 ? 
O12 B7 K4 155.3(3) 5_666 3_656 ? 
O24 B8 O28 122.6(5) . 5_666 ? 
O24 B8 O17 116.9(5) . . ? 
O28 B8 O17 120.3(5) 5_666 . ? 
O24 B8 K3 54.3(3) . . ? 
O28 B8 K3 146.6(4) 5_666 . ? 
O17 B8 K3 71.4(3) . . ? 
O26 B9 O21 122.3(5) . 5_666 ? 
O26 B9 O22 121.3(6) . . ? 
O21 B9 O22 116.4(5) 5_666 . ? 
O26 B9 K1 49.2(3) . 4_456 ? 
O21 B9 K1 132.8(4) 5_666 4_456 ? 
O22 B9 K1 90.8(4) . 4_456 ? 
O27 K1 O26 92.47(13) . 4_556 ? 
O27 K1 O4 172.80(14) . 8_755 ? 
O26 K1 O4 94.40(13) 4_556 8_755 ? 
O27 K1 O19 96.49(13) . . ? 
O26 K1 O19 86.42(13) 4_556 . ? 
O4 K1 O19 81.81(13) 8_755 . ? 
O27 K1 O17 80.97(15) . 7_566 ? 
O26 K1 O17 158.13(15) 4_556 7_566 ? 
O4 K1 O17 93.37(15) 8_755 7_566 ? 
O19 K1 O17 114.94(14) . 7_566 ? 
O27 K1 O1 99.20(13) . 8_755 ? 
O26 K1 O1 75.82(13) 4_556 8_755 ? 
O4 K1 O1 84.60(12) 8_755 8_755 ? 
O19 K1 O1 156.69(13) . 8_755 ? 
O17 K1 O1 84.61(13) 7_566 8_755 ? 
O27 K1 O2 132.13(12) . 8_755 ? 
O26 K1 O2 46.56(11) 4_556 8_755 ? 
O4 K1 O2 54.98(11) 8_755 8_755 ? 
O19 K1 O2 102.89(12) . 8_755 ? 
O17 K1 O2 126.38(13) 7_566 8_755 ? 
O1 K1 O2 53.86(11) 8_755 8_755 ? 
O27 K1 O6 45.54(11) . . ? 
O26 K1 O6 102.93(12) 4_556 . ? 
O4 K1 O6 130.23(12) 8_755 . ? 
O19 K1 O6 53.76(11) . . ? 
O17 K1 O6 87.38(12) 7_566 . ? 
O1 K1 O6 144.71(12) 8_755 . ? 
O2 K1 O6 146.19(11) 8_755 . ? 
O27 K1 B2 24.48(12) . . ? 
O26 K1 B2 88.52(13) 4_556 . ? 
O4 K1 B2 153.55(14) 8_755 . ? 
O19 K1 B2 72.13(13) . . ? 
O17 K1 B2 93.54(15) 7_566 . ? 
O1 K1 B2 121.47(13) 8_755 . ? 
O2 K1 B2 134.96(13) 8_755 . ? 
O6 K1 B2 25.05(11) . . ? 
O27 K1 B9 75.17(14) . 4_556 ? 
O26 K1 B9 21.38(14) 4_556 4_556 ? 
O4 K1 B9 112.01(14) 8_755 4_556 ? 
O19 K1 B9 100.67(15) . 4_556 ? 
O17 K1 B9 138.97(17) 7_566 4_556 ? 
O1 K1 B9 67.22(15) 8_755 4_556 ? 
O2 K1 B9 58.52(13) 8_755 4_556 ? 
O6 K1 B9 98.59(13) . 4_556 ? 
B2 K1 B9 78.03(15) . 4_556 ? 
O27 K1 B1 116.02(14) . 4_556 ? 
O26 K1 B1 23.97(12) 4_556 4_556 ? 
O4 K1 B1 71.01(13) 8_755 4_556 ? 
O19 K1 B1 88.34(14) . 4_556 ? 
O17 K1 B1 150.35(15) 7_566 4_556 ? 
O1 K1 B1 69.31(13) 8_755 4_556 ? 
O2 K1 B1 24.56(12) 8_755 4_556 ? 
O6 K1 B1 122.06(13) . 4_556 ? 
B2 K1 B1 111.76(14) . 4_556 ? 
B9 K1 B1 41.60(14) 4_556 4_556 ? 
O27 K1 B3 19.56(14) . . ? 
O26 K1 B3 107.17(15) 4_556 . ? 
O4 K1 B3 155.86(15) 8_755 . ? 
O19 K1 B3 109.67(14) . . ? 
O17 K1 B3 62.63(16) 7_566 . ? 
O1 K1 B3 90.19(13) 8_755 . ? 
O2 K1 B3 136.57(13) 8_755 . ? 
O6 K1 B3 55.94(12) . . ? 
B2 K1 B3 41.22(14) . . ? 
B9 K1 B3 87.30(16) 4_556 . ? 
B1 K1 B3 128.74(15) 4_556 . ? 
O1 K2 O20 139.01(15) . 6_657 ? 
O1 K2 O16 91.63(15) . 8_765 ? 
O20 K2 O16 129.30(16) 6_657 8_765 ? 
O1 K2 O24 89.57(14) . 2_665 ? 
O20 K2 O24 99.81(13) 6_657 2_665 ? 
O16 K2 O24 78.45(15) 8_765 2_665 ? 
O1 K2 O5W 79.3(2) . 6_657 ? 
O20 K2 O5W 62.7(2) 6_657 6_657 ? 
O16 K2 O5W 154.0(3) 8_765 6_657 ? 
O24 K2 O5W 125.3(3) 2_665 6_657 ? 
O1 K2 O7W 64.6(4) . . ? 
O20 K2 O7W 111.0(5) 6_657 . ? 
O16 K2 O7W 85.1(7) 8_765 . ? 
O24 K2 O7W 148.9(5) 2_665 . ? 
O5W K2 O7W 69.0(7) 6_657 . ? 
O1 K2 O6W 67.1(6) . 2_665 ? 
O20 K2 O6W 78.8(6) 6_657 2_665 ? 
O16 K2 O6W 141.4(6) 8_765 2_665 ? 
O24 K2 O6W 70.0(5) 2_665 2_665 ? 
O5W K2 O6W 56.3(6) 6_657 2_665 ? 
O7W K2 O6W 111.2(7) . 2_665 ? 
O1 K2 O15 133.81(14) . 6_657 ? 
O20 K2 O15 57.18(11) 6_657 6_657 ? 
O16 K2 O15 92.71(14) 8_765 6_657 ? 
O24 K2 O15 46.74(10) 2_665 6_657 ? 
O5W K2 O15 111.2(2) 6_657 6_657 ? 
O7W K2 O15 161.6(4) . 6_657 ? 
O6W K2 O15 81.7(4) 2_665 6_657 ? 
O1 K2 B4 108.64(15) . 2_665 ? 
O20 K2 B4 75.08(13) 6_657 2_665 ? 
O16 K2 B4 93.71(16) 8_765 2_665 ? 
O24 K2 B4 24.74(12) 2_665 2_665 ? 
O5W K2 B4 112.3(3) 6_657 2_665 ? 
O7W K2 B4 173.0(4) . 2_665 ? 
O6W K2 B4 65.9(4) 2_665 2_665 ? 
O15 K2 B4 25.18(12) 6_657 2_665 ? 
O1 K2 V3 145.95(13) . 6_657 ? 
O20 K2 V3 24.88(9) 6_657 6_657 ? 
O16 K2 V3 115.09(11) 8_765 6_657 ? 
O24 K2 V3 76.50(9) 2_665 6_657 ? 
O5W K2 V3 83.75(19) 6_657 6_657 ? 
O7W K2 V3 134.5(4) . 6_657 ? 
O6W K2 V3 78.9(5) 2_665 6_657 ? 
O15 K2 V3 32.31(7) 6_657 6_657 ? 
B4 K2 V3 52.01(10) 2_665 6_657 ? 
O1 K2 K3 50.91(11) . 2_665 ? 
O20 K2 K3 115.40(12) 6_657 2_665 ? 
O16 K2 K3 97.45(14) 8_765 2_665 ? 
O24 K2 K3 42.72(9) 2_665 2_665 ? 
O5W K2 K3 95.5(2) 6_657 2_665 ? 
O7W K2 K3 115.4(4) . 2_665 ? 
O6W K2 K3 44.0(6) 2_665 2_665 ? 
O15 K2 K3 82.95(9) 6_657 2_665 ? 
B4 K2 K3 57.85(11) 2_665 2_665 ? 
V3 K2 K3 102.37(7) 6_657 2_665 ? 
O1 K2 K4 138.25(13) . 6_657 ? 
O20 K2 K4 36.35(11) 6_657 6_657 ? 
O16 K2 K4 108.59(14) 8_765 6_657 ? 
O24 K2 K4 129.39(10) 2_665 6_657 ? 
O5W K2 K4 66.5(2) 6_657 6_657 ? 
O7W K2 K4 80.8(4) . 6_657 ? 
O6W K2 K4 108.5(7) 2_665 6_657 ? 
O15 K2 K4 82.65(9) 6_657 6_657 ? 
B4 K2 K4 106.09(11) 2_665 6_657 ? 
V3 K2 K4 54.70(5) 6_657 6_657 ? 
K3 K2 K4 150.70(8) 2_665 6_657 ? 
O24 K3 O8A 84.1(6) . . ? 
O24 K3 O11 139.51(14) . 2_664 ? 
O8A K3 O11 128.8(7) . 2_664 ? 
O24 K3 O6W 77.1(5) . . ? 
O8A K3 O6W 88.2(8) . . ? 
O11 K3 O6W 80.8(5) 2_664 . ? 
O24 K3 O4W 69.0(2) . 4_556 ? 
O8A K3 O4W 35.5(7) . 4_556 ? 
O11 K3 O4W 151.5(2) 2_664 4_556 ? 
O6W K3 O4W 114.3(5) . 4_556 ? 
O24 K3 O18 149.77(17) . 2_664 ? 
O8A K3 O18 70.0(6) . 2_664 ? 
O11 K3 O18 59.62(12) 2_664 2_664 ? 
O6W K3 O18 86.6(4) . 2_664 ? 
O4W K3 O18 95.8(2) 4_556 2_664 ? 
O24 K3 O3W 127.7(2) . 4_556 ? 
O8A K3 O3W 77.9(6) . 4_556 ? 
O11 K3 O3W 86.7(2) 2_664 4_556 ? 
O6W K3 O3W 149.1(5) . 4_556 ? 
O4W K3 O3W 68.0(2) 4_556 4_556 ? 
O18 K3 O3W 62.7(2) 2_664 4_556 ? 
O24 K3 O1 83.31(12) . 2_664 ? 
O8A K3 O1 153.6(6) . 2_664 ? 
O11 K3 O1 56.72(11) 2_664 2_664 ? 
O6W K3 O1 66.4(4) . 2_664 ? 
O4W K3 O1 150.6(2) 4_556 2_664 ? 
O18 K3 O1 113.39(13) 2_664 2_664 ? 
O3W K3 O1 127.8(2) 4_556 2_664 ? 
O24 K3 O17 46.14(12) . . ? 
O8A K3 O17 107.5(6) . . ? 
O11 K3 O17 122.23(15) 2_664 . ? 
O6W K3 O17 116.7(5) . . ? 
O4W K3 O17 74.3(2) 4_556 . ? 
O18 K3 O17 156.66(16) 2_664 . ? 
O3W K3 O17 94.0(2) 4_556 . ? 
O1 K3 O17 79.61(14) 2_664 . ? 
O24 K3 B8 23.69(13) . . ? 
O8A K3 B8 89.5(7) . . ? 
O11 K3 B8 141.62(16) 2_664 . ? 
O6W K3 B8 100.3(5) . . ? 
O4W K3 B8 62.5(2) 4_556 . ? 
O18 K3 B8 158.24(16) 2_664 . ? 
O3W K3 B8 107.0(2) 4_556 . ? 
O1 K3 B8 88.18(14) 2_664 . ? 
O17 K3 B8 24.66(13) . . ? 
O24 K3 O29 43.49(11) . . ? 
O8A K3 O29 54.9(6) . . ? 
O11 K3 O29 131.85(14) 2_664 . ? 
O6W K3 O29 51.4(5) . . ? 
O4W K3 O29 65.6(2) 4_556 . ? 
O18 K3 O29 106.78(14) 2_664 . ? 
O3W K3 O29 130.82(18) 4_556 . ? 
O1 K3 O29 100.98(12) 2_664 . ? 
O17 K3 O29 88.56(11) . . ? 
B8 K3 O29 64.11(12) . . ? 
O24 K3 O4 126.06(14) . 2_664 ? 
O8A K3 O4 130.4(6) . 2_664 ? 
O11 K3 O4 54.38(11) 2_664 2_664 ? 
O6W K3 O4 132.5(5) . 2_664 ? 
O4W K3 O4 112.9(2) 4_556 2_664 ? 
O18 K3 O4 83.59(13) 2_664 2_664 ? 
O3W K3 O4 52.58(17) 4_556 2_664 ? 
O1 K3 O4 75.33(13) 2_664 2_664 ? 
O17 K3 O4 81.18(13) . 2_664 ? 
B8 K3 O4 105.74(15) . 2_664 ? 
O29 K3 O4 169.55(12) . 2_664 ? 
O2W K4 O20 81.9(2) . . ? 
O2W K4 O28 118.3(3) . 3_646 ? 
O20 K4 O28 146.94(18) . 3_646 ? 
O2W K4 O3W 146.5(3) . . ? 
O20 K4 O3W 69.5(2) . . ? 
O28 K4 O3W 81.7(2) 3_646 . ? 
O2W K4 O22 64.3(2) . 6_657 ? 
O20 K4 O22 136.78(18) . 6_657 ? 
O28 K4 O22 75.85(15) 3_646 6_657 ? 
O3W K4 O22 149.1(2) . 6_657 ? 
O2W K4 O11W 99.4(4) . 2_665 ? 
O20 K4 O11W 92.9(3) . 2_665 ? 
O28 K4 O11W 107.9(3) 3_646 2_665 ? 
O3W K4 O11W 99.1(4) . 2_665 ? 
O22 K4 O11W 68.7(4) 6_657 2_665 ? 
O2W K4 O3 66.5(3) . . ? 
O20 K4 O3 90.53(15) . . ? 
O28 K4 O3 76.15(14) 3_646 . ? 
O3W K4 O3 95.8(2) . . ? 
O22 K4 O3 99.04(18) 6_657 . ? 
O11W K4 O3 164.9(4) 2_665 . ? 
O2W K4 O30 113.8(2) . 7_566 ? 
O20 K4 O30 154.02(19) . 7_566 ? 
O28 K4 O30 44.41(11) 3_646 7_566 ? 
O3W K4 O30 99.3(2) . 7_566 ? 
O22 K4 O30 49.82(12) 6_657 7_566 ? 
O11W K4 O30 65.0(3) 2_665 7_566 ? 
O3 K4 O30 114.42(14) . 7_566 ? 
O2W K4 B7 128.0(2) . 3_646 ? 
O20 K4 B7 150.2(2) . 3_646 ? 
O28 K4 B7 24.11(12) 3_646 3_646 ? 
O3W K4 B7 81.6(2) . 3_646 ? 
O22 K4 B7 69.23(15) 6_657 3_646 ? 
O11W K4 B7 84.0(3) 2_665 3_646 ? 
O3 K4 B7 100.12(15) . 3_646 ? 
O30 K4 B7 24.21(11) 7_566 3_646 ? 
O2W K4 V3 72.8(2) . . ? 
O20 K4 V3 22.44(9) . . ? 
O28 K4 V3 133.92(14) 3_646 . ? 
O3W K4 V3 74.24(19) . . ? 
O22 K4 V3 136.56(16) 6_657 . ? 
O11W K4 V3 114.3(3) 2_665 . ? 
O3 K4 V3 68.11(11) . . ? 
O30 K4 V3 173.45(14) 7_566 . ? 
B7 K4 V3 151.48(14) 3_646 . ? 
O2W K4 V2 64.6(2) . . ? 
O20 K4 V2 68.20(11) . . ? 
O28 K4 V2 95.69(13) 3_646 . ? 
O3W K4 V2 88.14(18) . . ? 
O22 K4 V2 114.75(16) 6_657 . ? 
O11W K4 V2 156.1(3) 2_665 . ? 
O3 K4 V2 22.33(9) . . ? 
O30 K4 V2 136.56(12) 7_566 . ? 
B7 K4 V2 119.70(13) 3_646 . ? 
V3 K4 V2 45.78(5) . . ? 
O2W K4 K2 65.4(2) . 6_557 ? 
O20 K4 K2 36.55(10) . 6_557 ? 
O28 K4 K2 173.26(16) 3_646 6_557 ? 
O3W K4 K2 98.0(2) . 6_557 ? 
O22 K4 K2 101.88(13) 6_657 6_557 ? 
O11W K4 K2 65.5(3) 2_665 6_557 ? 
O3 K4 K2 110.56(13) . 6_557 ? 
O30 K4 K2 129.42(12) 7_566 6_557 ? 
B7 K4 K2 149.16(15) 3_646 6_557 ? 
V3 K4 K2 51.78(5) . 6_557 ? 
V2 K4 K2 91.02(7) . 6_557 ? 
O5W K5 O3W 93.9(3) . . ? 
O5W K5 O20 65.8(3) . . ? 
O3W K5 O20 70.3(2) . . ? 
O5W K5 O4W 151.8(3) . . ? 
O3W K5 O4W 69.5(3) . . ? 
O20 K5 O4W 124.5(2) . . ? 
O5W K5 O23 146.1(3) . . ? 
O3W K5 O23 73.7(2) . . ? 
O20 K5 O23 80.33(13) . . ? 
O4W K5 O23 52.6(2) . . ? 
O5W K5 O14 109.9(3) . . ? 
O3W K5 O14 104.3(2) . . ? 
O20 K5 O14 59.13(12) . . ? 
O4W K5 O14 96.5(2) . . ? 
O23 K5 O14 47.06(10) . . ? 
O5W K5 O17 88.6(3) . 4_456 ? 
O3W K5 O17 100.7(2) . 4_456 ? 
O20 K5 O17 151.47(17) . 4_456 ? 
O4W K5 O17 73.1(2) . 4_456 ? 
O23 K5 O17 124.26(15) . 4_456 ? 
O14 K5 O17 147.39(18) . 4_456 ? 
O5W K5 O26 143.7(3) . . ? 
O3W K5 O26 115.6(2) . . ? 
O20 K5 O26 103.26(14) . . ? 
O4W K5 O26 63.7(2) . . ? 
O23 K5 O26 43.09(11) . . ? 
O14 K5 O26 44.89(11) . . ? 
O17 K5 O26 104.95(15) 4_456 . ? 
O5W K5 B1 137.1(3) . . ? 
O3W K5 B1 97.4(2) . . ? 
O20 K5 B1 79.46(15) . . ? 
O4W K5 B1 69.6(2) . . ? 
O23 K5 B1 25.45(13) . . ? 
O14 K5 B1 27.19(12) . . ? 
O17 K5 B1 129.04(17) 4_456 . ? 
O26 K5 B1 26.14(12) . . ? 
O5W K5 V3 89.0(2) . . ? 
O3W K5 V3 79.1(2) . . ? 
O20 K5 V3 26.26(9) . . ? 
O4W K5 V3 109.0(2) . . ? 
O23 K5 V3 58.03(9) . . ? 
O14 K5 V3 34.31(8) . . ? 
O17 K5 V3 177.62(14) 4_456 . ? 
O26 K5 V3 77.19(10) . . ? 
B1 K5 V3 53.27(11) . . ? 
O5W K5 K3 105.4(3) . 4_456 ? 
O3W K5 K3 51.0(2) . 4_456 ? 
O20 K5 K3 120.39(17) . 4_456 ? 
O4W K5 K3 46.39(19) . 4_456 ? 
O23 K5 K3 91.20(12) . 4_456 ? 
O14 K5 K3 138.18(13) . 4_456 ? 
O17 K5 K3 52.37(11) 4_456 4_456 ? 
O26 K5 K3 109.52(12) . 4_456 ? 
B1 K5 K3 113.81(15) . 4_456 ? 
V3 K5 K3 128.12(12) . 4_456 ? 
O5W K5 K4 67.3(3) . . ? 
O3W K5 K4 37.5(2) . . ? 
O20 K5 K4 35.89(11) . . ? 
O4W K5 K4 104.9(2) . . ? 
O23 K5 K4 85.44(12) . . ? 
O14 K5 K4 88.57(11) . . ? 
O17 K5 K4 123.80(15) 4_456 . ? 
O26 K5 K4 124.78(12) . . ? 
B1 K5 K4 98.78(14) . . ? 
V3 K5 K4 54.80(7) . . ? 
K3 K5 K4 84.94(10) 4_456 . ? 
K5 O3W K4 106.1(3) . . ? 
K5 O3W K3 83.9(3) . 4_456 ? 
K4 O3W K3 149.4(3) . 4_456 ? 
O8A O4W K3 72.3(11) 4_456 4_456 ? 
O8A O4W K5 141.5(11) 4_456 . ? 
K3 O4W K5 83.9(3) 4_456 . ? 
K3 O6W K2 84.5(6) . 2_664 ? 
K5 O5W K2 104.8(3) . 6_557 ? 
O12W O11W K4 148.7(18) 5_766 2_664 ? 
O4W O8A K3 72.2(11) 4_556 . ? 
 
_diffrn_measured_fraction_theta_max    0.999 
_diffrn_reflns_theta_full              26.50 
_diffrn_measured_fraction_theta_full   0.999 
_refine_diff_density_max    2.275 
_refine_diff_density_min   -2.300 
_refine_diff_density_rms    0.197 
